Experimental study on behavior of mortar-aggregate interface after elevated temperatures
- 83 Downloads
A push-out test program was designed and conducted to study the meso-scale behavior of mortar-aggregate interface for concrete after elevated temperatures ranging from 20°C to 600°C with the concept of modeled concrete (MC) and modeled recycled aggregate concrete (MRAC). The MCs and MRACs were designed with different strength grade of mortar and were exposed to different elevated temperatures. Following that the specimens were cooled to room temperature and push-out tests were conducted. Failure process and mechanical behaviors were analyzed based on failure modes, residual load-displacement curves, residual peak loads and peak displacements. It is found that failure modes significantly depended on specimen type, the elevated temperature and the strength grade of mortar. For MC, major cracks started to propagate along the initial cracks caused by elevated temperatures at about 80% of residual peak load. For MRAC, the cracks appeared at a lower level of load with the increasing elevated temperatures. The cracks connected with each other, formed a failure face and the specimens were split into several parts suddenly when reaching the residual peak load. Residual load-displacement curves of different specimens had similarities in shape. Besides, effect of temperatures and strength grade of mortar on residual peak load and peak displacement were analyzed. For MC and MRAC with higher strength of new hardened mortar, the residual peak load kept constant when the temperature is lower than 400°C and dropped by 43.5% on average at 600°C. For MRAC with lower strength of new hardened mortar, the residual peak load began to reduce when the temperatures exceeded 200°C and reduced by 27.4% and 60.8% respectively at 400°C and 600°C. The properties of recycled aggregate concrete (RAC) may be more sensitive to elevated temperatures than those of natural aggregate concrete (NAC) due to the fact that the interfacial properties of RAC are lower than those of NAC, and are deteriorated at lower temperatures.
Keywordsmortar-aggregate interface push-out test elevated temperatures modeled concrete (MC) modeled recycled aggregate concrete (MRAC)
Unable to display preview. Download preview PDF.
The authors would like to gratefully acknowledge the research grants from the Chinese National 973 Plan (Grant No. 2012CB719703).
- 2.Rostasy F S, Hinrichsmeyer K. Structural alterations in concrete due to thermal and mechanical stresses. In: Proceedings of the International Conference on Materials Science to Construction Materials Engineering. Cersailles, 1987Google Scholar
- 3.Sideny M, Young J F, Darwin D. Concrete. Translated by Wu K, Zhang X, Yao W, et al. Beijing: Chemical Industry Press, 2005Google Scholar
- 5.Mehta P K, Monteiro P J M. Concrete structure properties and materials. 2nd ed. Englewood Cliffs: prentice Hall, 1993Google Scholar
- 13.Shah S P, Winter G. Inelastic behavior and fracture of concrete. ACI Special Publications, 1968, 20: 5–28Google Scholar
- 14.Buyukozturk O, Nilson A H, Slate F O. Stress-strain response and fracture of concrete in biaxial loading. ACI Journal Proceedings, 1971, 68: 590–599Google Scholar
- 15.Xiao J Z, LiWG, Sun Z H, Shah S P. Crack propagation in recycled aggregate concrete under uniaxial compressive loading. ACI Materials Journal, 2012, 109(4): 451–461Google Scholar
- 22.Piasta J, Sawicz Z, Rudzinski L. Changes in the structure of hardened cement paste due to high temperature. Materiales de Construcciin, 1984, 17(4): 291–296Google Scholar
- 26.Lin W M, Lin T D, Powers-Couche L J. Microstructures of firedamaged concrete. ACI Materials Journal, 1996, 93(3): 199–205Google Scholar